Author
truongdung
View
218
Download
0
Embed Size (px)
Contents lists available at ScienceDirect
Journal of the Mechanics and Physics of Solids
Journal of the Mechanics and Physics of Solids 66 (2014) 4258
http://d0022-50
n CorrE-m
journal homepage: www.elsevier.com/locate/jmps
Thermomechanics of monolayer graphene: Rippling, thermalexpansion and elasticity
Wei Gao, Rui Huang n
Department of Aerospace Engineering and Engineering mechanics, University of Texas, Austin, TX 78712, USA
a r t i c l e i n f o
Article history:Received 15 September 2013Received in revised form1 December 2013Accepted 28 January 2014Available online 15 February 2014
Keywords:GrapheneThermal expansionElasticityMolecular dynamicsStatistical mechanics
x.doi.org/10.1016/j.jmps.2014.01.01196 & 2014 Elsevier Ltd. All rights reserved.
esponding author.ail address: [email protected] (R. Hu
a b s t r a c t
Thermomechanical properties of monolayer graphene with thermal fluctuation are studiedby both statistical mechanics analysis and molecular dynamics (MD) simulations. While thestatistical mechanics analysis in the present study is limited by a harmonic approximation,significant anharmonic effects are revealed by MD simulations. The amplitude of out-of-plane thermal fluctuation is calculated for graphene membranes under both zero stress andzero strain conditions. It is found that the fluctuation amplitude follows a power-law scalingwith respect to the linear dimension of the membrane, but the roughness exponents aredifferent for the two conditions due to anharmonic interactions between bending andstretching modes. Such thermal fluctuation or rippling is found to be responsible for theeffectively negative in-plane thermal expansion of graphene at relatively low temperatures,while a transition to positive thermal expansion is predicted as the anharmonic interactionssuppress the rippling effect at high temperatures. Subject to equi-biaxial tension, theamplitude of thermal rippling decreases nonlinearly, and the in-plane stress-strain relationof graphene becomes nonlinear even at infinitesimal strain, in contrast with classical theoryof linear elasticity. It is found that the tangent biaxial modulus of graphene depends onstrain non-monotonically, decreases with increasing temperature, and depends on mem-brane size. Both statistical mechanics and MD simulations suggest considerable entropiccontribution to the thermomechanical properties of graphene, and as a result thermalrippling is intricately coupled with thermal expansion and thermoelasticity for monolayergraphene membranes.
& 2014 Elsevier Ltd. All rights reserved.
1. Introduction
As a two-dimensional crystal membrane, graphene has drawn tremendous interests for research and applications. Among itsmany unique properties, the mechanical properties of graphene combine high in-plane stiffness and high strength (Lee et al.,2008) with extremely low flexural stiffness (Lu et al., 2009), rendering a highly deformable but robust membrane material.Experimental observations have found that suspended graphene membranes often display spontaneous ripples (Meyer et al.,2007; Bangert et al., 2009; Zan et al., 2012). Theoretically, different physical origins for rippling have been proposed. Thompson-Flagg et al. (2009) suggested that the rippling could be a consequence of adsorbed OH molecules on random sites. On the otherhand, thermal fluctuation has been considered as a reasonable explanation for intrinsic ripples in graphene (Fasolino et al., 2007;
ang).
www.sciencedirect.com/science/journal/00225096www.elsevier.com/locate/jmpshttp://dx.doi.org/10.1016/j.jmps.2014.01.011http://dx.doi.org/10.1016/j.jmps.2014.01.011http://dx.doi.org/10.1016/j.jmps.2014.01.011http://crossmark.crossref.org/dialog/?doi=10.1016/j.jmps.2014.01.011&domain=pdfhttp://crossmark.crossref.org/dialog/?doi=10.1016/j.jmps.2014.01.011&domain=pdfhttp://crossmark.crossref.org/dialog/?doi=10.1016/j.jmps.2014.01.011&domain=pdfhttp://dx.doi.org/10.1016/j.jmps.2014.01.011
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 4258 43
Abedpour et al., 2007). In the present study, we focus on the effects of thermal fluctuation on thermomechanical properties ofmonolayer graphene, including thermal expansion and temperature-dependent elastic modulus.
The basic mechanical properties of graphene have been reasonably understood, including elastic moduli for in-planeextension and bending. However, the effect of temperature on the mechanical properties of graphene is not well understood.The fact that the elastic moduli measured at the room temperature (T300 K) are in close agreement with theoretical valuespredicted at T0 K may imply insignificant temperature dependence for the elastic moduli. By molecular dynamics (MD)simulations, Zhao and Aluru (2010) predicted that Young's modulus of graphene does not vary significantly with temperatureup to about 1200 K, beyond which graphene becomes more compliant. On the other hand, by means of atomistic Monte Carlo(MC) simulations, Zakharchenko et al. (2009) predicted a non-monotonic behavior of shear modulus of graphene with amaximum at about 900 K, and Chen and Chrzan (2011) predicted monotonic decrease of the elastic modulus of graphenewith temperature up to 4000 K. Since graphene spontaneously fluctuates out-of-plane at a finite temperature, the effective in-plane elastic modulus is expected to depend on the significance of thermal fluctuation. Another manifestation of out-of-planethermal fluctuation is possible reduction of the projected area, which has been suggested as the cause for negative in-planethermal expansion of graphene (Zakharchenko et al., 2009; Chen and Chrzan, 2011). Based on density-functional-theory (DFT)calculations and a quasiharmonic approximation (QHA), Mounet and Marzari (2005) predicted negative in-plane thermalexpansion for graphite and graphene, which was attributed to the lowest transversal acoustic (ZA) phonon modes (also calledbending modes). Negative thermal expansion of graphene was also predicted by a nonequilibrium Green's function approach(Jiang et al., 2009) and ab initio molecular dynamics (AIMD) simulations (Pozzo et al., 2011). Experimentally, Bao et al. (2009)measured thermal expansion of suspended graphene by SEM imaging between 300 and 400 K, with a transition from negativeto positive coefficient of thermal expansion (CTE). Based on frequency measurements of suspended graphene electromecha-nical resonators, Singh et al. (2010) extracted negative CTEs for graphene between 300 and 30 K. Considerable discrepanciesremain between the experimental measurements and theoretical predictions for CTE of graphene.
The present work combines MD simulations of graphene with a statistical mechanics (SM) approach for the study ofthermomechanical properties of monolayer graphene. The SM approach has been used extensively for the study of flexiblemembranes (Bowick and Travesset, 2001; Nelson et al., 2004; Freund, 2013), primarily for biological membranes. Withrelatively simple atomistic structures in graphene, it is possible to directly sample the statistical behavior of graphenemembranes with atomistic details to compare with theoretical SM analysis (Los et al., 2009; Zakharchenko et al., 2010),hence opening a new paradigm for the study of membrane physics. The rest of this paper is organized as follows.A theoretical approach based on statistical mechanics of a continuum elastic membrane is presented in Section 2. Section 3describes the MD simulation method. In Section 4, the results from MD simulations are discussed in comparison with thetheoretical analysis. Section 5 summarizes the results and findings.
2. Statistical mechanics of graphene
2.1. A continuum membrane model
Consider monolayer graphene as a continuum membrane with a two-dimensional (2D) reference configuration in theground state at T0 K. The in-plane dimensions of the graphene membrane are much larger than the atomic length scales(e.g., the bond length, r00.142 nm), while the monatomic thickness is undefined (and unnecessary) in the continuummodel. The kinematics of general thermomechanical deformation can be described by an in-plane GreenLagrange straintensor and a curvature tensor, based on a 2D to 3D mapping (Arroyo and Belytschko, 2002; Lu and Huang, 2009). Under theassumption of relatively small deformation but with moderately large out-of-plane deflection, the in-plane strain andcurvature are approximately
12
ux
ux
wx
wx
; 1
and
2w
xx; 2
where the Greek subscript ( or ) represents x or y for the in-plane coordinates, ux and uy are in-plane displacements, and w isout-of-plane deflection. It is noted that the strain tensor in Eq. (1) includes a nonlinear contribution from the out-of-planedeflection that leads to geometric coupling between the in-plane and out-of-plane deformation modes. The kinematics isidentical to the von Karman nonlinear plate theory (Timoshenko and Woinowsky-Krieger, 1987).
The total potential energy of the membrane consists of two parts: in-plane strain energy and bending energy. Under thecondition of small deformation, the strain energy density function can be written as
; ; 3
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 425844
where
E21
1
; 4
12DI2 DGII
DDG2
DG2
: 5
Four elastic constants are used in the above equations, including the 2D Young's modulus E (unit: N/m), Poisson's ratio ,bending modulus D, and Gaussian curvature modulus DG. They are all defined for the potential energy in the ground state,thus independent of temperature. Note that the bending strain energy density is written as a function of the twoinvariants of the curvature tensor (Helfrich, 1973): I 1122 and II 1122212; the first invariant is twice of the meancurvature, and the second invariant is Gaussian curvature. In classical plate theory (Timoshenko and Woinowsky-Krieger,1987), both bending moduli (D and DG) can be related to the in-plane Young's modulus and Poisson's ratio. For graphene,however, they are determined from atomistic modeling as independent constants (Koskinen and Kit, 2010; Wei et al., 2012).As discussed in a previous study (Lu et al., 2009), the physical origin of the bending moduli of monolayer graphene isfundamentally different from that in classical plate theory.
As noted by Helfrich (1973) in the study of lipid bilayers, the bending energy due to Gaussian curvature depends solelyon boundary conditions and can be ignored in most cases. Therefore, the total bending energy of a membrane can be writtenas an area integral:
Ub
dxdyD2
2wx2
2wy2
2dxdy 6
where is the area of the membrane in the reference state. In the present work, we extend the Helfrich membrane modelto study thermomechanical properties of graphene, in comparison with MD simulations.
The mechanical properties of graphene in the ground state (T0 K) have been predicted by DFT calculations (Kudin et al.,2001): E345 N/m, 0.15, and D1.5 eV. However, the empirical potential used in the MD simulations yields differentvalues (Lu and Huang, 2009): E243 N/m, 0.397, and D1.4 eV. The second set of mechanical properties is used whencomparing the theoretical predictions with MD simulations. Despite the discrepancy in the 2D Young's modulus, thepredictions for the 2D biaxial modulus, En E=1, are in close agreement between the empirical potential (En403 N/m)and DFT (En406 N/m).
2.2. Out-of-plane thermal fluctuation
Now consider a square-shaped graphene membrane of side length L0 in the ground state. At a finite temperature butsubject to no external force, the membrane fluctuates with both in-plane and out-of-plane modes. In this section weconsider out-of-plane thermal fluctuation only. Assuming periodic boundary conditions, the lateral deflection can be writtenin form of the Fourier series:
wr kwqkeiqk U r; 7
and the Fourier coefficients are
wqk 1
L20
wre iqk U rd; 8
where r is the 2D position vector in the ground state and qk denotes the k-th wave vector in the 2D space.Substituting Eqs. (7) into (6) and applying the Parseval theorem (Kammler, 2007), we obtain the bending energy of the
membrane in terms of the Fourier coefficients
Ub DL202
kq4k w2Reqkw2Imqk; 9
where qk jqkj, wReqk and wImqk are the real and imaginary parts of wqk, respectively.For a statistical treatment, wReqk and wImqk are taken as continuous random variables. Each set of wReqk and wImqk
constitutes a possible configuration of the membrane. All possible configurations of the membrane construct a statisticalensemble. It is important to note that the Fourier coefficients wqk and wqk are not independent. Since w(r) is real-valued in Eq. (8), it can be shown that
wReqk wReqk and wImqk wImqk: 10
Consequently, only those Fourier coefficients associated with the upper half-plane of the wave vectors (i.e., qk UeyZ0,including only half of the x-axis) are taken as independent random variables. It then follows that the bending energy in
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 4258 45
Eq. (9) can be written in terms of the independent random variables as
Ub DL20 kqk Uey Z0
q4k w2Reqkw2Imqk
h i; 11
where ey is the unit vector in the positive direction of y-coordinate.For each possible configuration, the total potential energy is
U
;dUbUs 12
where Us d. Under the assumption of small deflection, the nonlinear contribution to the in-plane strain in Eq. (1)is neglected. Consequently, the in-plane strain energy Us is independent of the out-of-plane fluctuation, and the in-planeand out-of-plane modes are decoupled. This is commonly taken as a harmonic approximation.
Based on classical statistical mechanics (Pathria, 1996; Weiner, 2002), the probability density function (PDF) for eachconfiguration is given by Boltzmann distribution at thermal equilibrium:
1Zexp U
kBT
; 13
where kB is the Boltzmann constant, T is the temperature, and Z is the configurational partition function. The partitionfunction is calculated by an integral with respect to all independent random variables (including both the in-plane and out-of-plane modes) for all possible configurations. Under the harmonic approximation, the partition function is simply aproduct of two parts, namely
Z ZbZs; 14
where the contribution due to the out-of-plane modes is
Zb Z 11
Z 11
exp UbkBT
dwReq1dwImq1dwReq2dwImq2
kqk Uey Z0
Z 11
Z 11
exp DL20
kBTq4k w2Reqkw2Imqk
" #dwReqkdwImqk
kqk Uey Z0
kBT
DL20q4k
!15
and Zs is due to the in-plane modes (independent of the out-of-plane fluctuation). The range of each random variable in Eq.(15) has been taken to be from 1 to1 in order to obtain the analytical expression for the partition function. However, theformulation of the bending energy in Eq. (6) assumes moderately large deflection, requiring the fluctuation amplitude to beless than a fraction of its wavelength for each Fourier mode. Nevertheless, Eq. (15) offers a simple but reasonableapproximation, considering that the exponential integrant decays rapidly with the variables. In other words, the large-amplitude fluctuations are statistically suppressed due to the large potential energy (hence low probability density).
With the probability density function in Eq. (13), the mean-square of each Fourier coefficient of the out-of-planefluctuation can be calculated as
jwqkj21Zb
Z 11
Z 11
jwqkj2exp UbkBT
dwReq1dwImq1
kBT
DL20q4k
: 16
Alternatively, by the equi-partition theorem (Pathria, 1996), each independent harmonic term in Eq. (11) has an averageenergy of kBT/2, namely
DL20q4kw
2ReqkDL20q4kw
2Imqk
kBT2
; 17
which leads to the same result as Eq. (16).For each possible configuration, the mean-square amplitude of the out-of-plane fluctuation in the real space is
h2 1L20
w2rdkjwqkj2: 18
Therefore, the expectation value of the mean-square amplitude is
h2kjwqkj2
kBT
DL20kq4k : 19
For the square-shaped membrane with periodic boundary conditions, the smallest possible wave number is:qmin 2=L0, which depends on the membrane size (L0). The summation in Eq. (19) can then be written in a discrete
0 20 40 60 80 10010-2
10-1
100
101
n = L0/b
*n
0 = 0.1%
0 = 0
0 = 1%
0 0.5 1 1.5 2
10-1
100
101
0 (%)
*
5 nm10 nm20 nm
-1.5 -1 -0.5 0 0.5 1 1.50
50
100
150
200
250
300
350
400
Normalized strain
T (K
)anharmonic
harmonic
hc/L0 = 0.005
Tc
c
Fig. 1. (a) Convergence of the double-series summations in Eqs. (20) and (28), in comparison with the integral approximation (dashed lines) in Eqs. (21)and (29) for L020 nm; (b) dependence of the coefficient n1 on pre-strain for different membrane sizes (dashed lines by integration); (c) effect of pre-strain on RMS amplitude of out-of-plane thermal fluctuation at T300 K by harmonic analysis (symbols by summation and lines by integration); (d)critical temperature as a function of the normalized pre-strain, EnL200=4
2D, for the limit of harmonic analysis.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 425846
form as
h2 kBTDL20
L02
4n
i; j ni2 j240
i2 j22 nkBT164D
L20; 20
where n is a dimensionless coefficient and n qmax=qmin L0=b, with qmax 2=b being the largest possible wave numberand b the smallest physically permissible length scale (e.g., a microscopic cut-off). Alternatively, Helfrich and Servuss (1984)suggested that the summation in Eq. (19) can be converted to an integral as a continuum approximation:
h2 L02
2 Z qmaxqmin
kBT
DL20
1q4
!2qdq kBT
163DL20; 21
where L0bb has been assumed to simplify the result. A comparison between Eqs. (20) and (21) would lead to n- forn-1. However, as shown in Fig. 1a, the discrete summation in Eq. (20) converges to a larger value, n-6:026 (for zerostrain), nearly twice of the integral approximation. The discrepancy results from the singular behavior of q4k as qk-0.
As a typical measure of surface roughness, the root-mean-square (RMS) amplitude of the out-of-plane fluctuation isobtained as
hffiffiffiffiffiffiffiffiffih2
q L0
ffiffiffiffiffiffiffiffiffiffiffiffiffiffinkBT164D
r; 22
which scales linearly with the dimension (L0) of the membrane. Similar results were obtained for thermal fluctuation of fluidmembranes (Helfrich and Servuss, 1984). A slightly different derivation is presented here as an introduction to key conceptsin statistical mechanics. Notably, the constant coefficient in Eq. (21) differs from that in Helfrich and Servuss (1984) by afactor of 4, since the integral is evaluated with different limits for the wave number, following the assumption of periodicboundary conditions. Moreover, the integral approximation in Eq. (21) is found to be inaccurate to evaluate the discretesummation in Eq. (20) for the amplitude of out-of-plane fluctuation, although the linear scaling (hpL0) is unaffected.
W. Gao, R. Huang / J. Mech. Phys. Solids 66 (2014) 4258 47
2.3. Effect of pre-strain
Next we consider thermal fluctuation of a graphene membrane subjected to a biaxial pre-strain 0, relative to thereference ground state. In addition to the bending energy, the in-plane stretching energy is
Us
En20En02
wx
2 w
y
2" # E
n
81vwx
2 w
y
2" #28